Carbon nanotubes (CNTs), a novel carbonaceous material, have been widely studied since their discovery in 1991. CNTs have highly unique electronic, mechanical, catalytic, adsorption, and transport properties, making them interesting for a variety of applications. It is very important for the use of CNTs to prepare CNTs with various constructs in large scale and ideal quality. Up to now, CNTs have been produced by various kinds of strategies, mainly including Arc discharge, laser ablation, and chemical vapor deposition (CVD). Compared with the other two methods, CVD is considered as the most promising method for easily scaled-up to batch-scale production duo to simplicity and economy. At present, a lot of modified CVD were studied and explored for preparing pure CNTs in large scale, especially single-walled CNTs (SWCNTs), such as plasma-enhanced CVD (PECVD) and thermal CVD. A vapor–liquid–solid (VLS) mechanism is generally accepted for CNTs growth, and catalyst plays an important role in the CVD synthesis of CNTs, which is needed to be removed in follow purity of CNTs for further use. To avoid the problem, some modified CVD methods without metal particles as catalyst were also carried out for producing relative pure CNTs.
CNTs possess large speciﬁc surface areas due to their high aspect ratio, while their structural integrity and chemical inertness support relatively high oxidation stability in comparison with graphite. For these reasons, CNTs are promising building blocks for hybrid materials, which could endow CNTs more excellent performances for widely potential fields. CNTs-based hybrid materials, including CNTs-inorganic species and CNTs-organic species, were synthesized by numerous diverse strategies, which can be classed roughly into two kinds: ex situ approach (attaching nanoparticles to CNTs) and in situ synthesis (Directly on the CNTs surface). CNTs/metal oxide heterostructures are an important kind of CNTs-inorganic composites. The synergistic effect of CNTs and metal oxide makes CNTs/metal oxide heterostructures possess the properties of the both and have more widely potential application. The electrochemical properties of the CNTs/metal oxide heterostructures have attracted researchers’ interest duo to their excellent performances on electrochemical catalyst, electrochemical sensor, supercapacitors and batteries. Over the past few years a great number of CNTs/metal oxide heterostructures, such as TiO2/CNTs, Co3O4/CNTs, Au/CNTs, Au/TiO2/CNTs, Co/CoO/Co3O4/CNTs (Fig. 1)  etc, were synthesized and their electrochemical properties were investigated as well.
Numerous synthetic methodologies have been developed for the preparation of CNTs and their composites. In this chapter, besides the preparation of nanocomposites based on CNTs, we also focus on investigating the electrochemical applications of CNT/metal-oxide or hydroxide composites.
2. Synthesis of CNTs
CNTs with tubular structures are made entirely of rolled-up layers of interconnected carbon atoms [2,3], and with diameters ranging from about one nanometer to tens of nanometers and lengths up to centimeters. CNTs can be open-ended or closed by a hemispherical fullerene-type cap, depending on their synthesis method . CNTs have highly unique electronic, mechanical, catalytic, adsorption, and transport properties, making them interesting for a variety of applications [5-13]. The scale-up preparation of CNTs with high purity and homogeneity is essential for the use of CNTs in reality. In several past decades, a lot of effort was made to investigate the synthesis strategies of CNTs and modify constantly the promising methods. By far, various strategies, maily including Arc discharge, laser ablation, and various chemical vapor depositions (CVD), have been found to produce SWCNTs and MWCNTs with different merit and demerit. In this section, a brief discussion about the progress in preparation of CNTs is divided into two parts (synthesis of SWCNTs and synthesis of MWCNTs) and made.
2.1. Synthesis of SWCNTs
SWCNT can be considered to be a unique molecule, with different physical properties, depending on their chirality, which determines that SWCNTs are primarily metallic or semiconducting. Although obtaining a single aliquot of one (
SWCNTs were ﬁrst synthesized by the coevaporation of a cobalt catalyst and graphite in an electric arc [3,14]. In the early arc-generated nanotube material, the SWCNT ﬁbers typically consisted of 7-14 bundled SWCNTs, with the individual tubes being 1.0-1.5 nm in diameter. The early arc-generated materials also contained relatively low weight percent densities of SWCNTs. An improvement in the nanotube yield was observed by changing the metal catalysts employed in the arc-technique . Fig. 2a displays a transmission electron microscope (TEM) image of a typical arc SWCNT material generated with an iron catalyst . Note that the nanotube bundles are relatively small (containing~3-5 nanotubes). SWCNTs were later produced at much higher yield by the method of laser vaporization . Crystalline ropes micrometers in length containing 10-100 s of individual SWCNTs were easily obtained . Fig. 2b shows a typical TEM image of crude laser-generated material produced with an Alexandrite laser operating at ~45 W/cm2, with Co and Ni at 0.6 % each and an external furnace temperature of 1200 °C . Note the large, very long bundles of SWCNTs present in Fig. 2b. Although there is a high density of SWCNTs (30-40 wt %), non-nanotube carbon impurities, as well as metal catalyst particles, are still clearly visible in the TEM image. Laser-generated SWCNTs typically have low defect concentrations , making them easier to purify, since they are not as likely to be destroyed by the acids generally employed to remove metal catalyst particles. For example, Laser-genrated SWCNTs were puriﬁed with dilute HNO3 to remove the metal catalyst particles and then burned in air at 550 °C to remove the non-nanotube carbon . However, the laser technique is often considered to be too expensive to be industrially scalable.
Consequently, numerous research groups have turned to the development of CVD as a potentially low-cost scalable technique for the production of SWCNTs. In 1996, SWCNT growth employing CVD on a supported catalyst was demonstrated as a promising route to carbon nanotube production . Multiple reports quickly followed, further establishing CVD as a viable large-scale production process [23-32]. Typically, CVD materials contain more metal and often smaller and shorter SWCNT bundles than those produced in the laser processes. Fig. 2c shows a TEM image of commercially available CVD material produced by a high pressure carbon monoxide (HiPCO) process . CVD production of isolated nanotubes has been achieved on oxidized silicon substrates using an iron catalyst . Additionally, isolated SWCNTs have been generated in the gas phase by the technique of hot wire chemical vapor deposition (HWCVD) . Fig. 2d shows high-resolution TEM images of isolated SWCNTs produced by this HWCVD process. For comparison, a high resolution TEM image of a bundle of puriﬁed laser-generated SWCNTs is also provided in Fig. 2e . A multistep process for the puriﬁcation of HiPCO CVD-generated nanotubes was reported in 2001 . Recently, K. E. Hurst reported a simple“laser cleaning” method than can be employed to purify a host of CNT materials . The unavoidable metal species remaining in the SWCNT products would result in obvious disadvantages for both intrinsic property characterization and application exploration of SWCNTs. Despite sustained efforts, it has been until now an intractable problem to remove metal catalysts completely from SWCNT samples without introducing defects and contaminations. Surprisingly, in 2009, Liu et al. proposed a simple and effective method for growing SWCNTs via a metal-catalyst-free CVD process on a sputtering deposited SiO2 ﬁlm. Metal-free, pure, and dense SWCNTs were obtained . The successful growth of SWCNTs using a nonmetal catalyst can provide valuable implications for understanding the growth mechanism of SWCNTs in-depth, which accordingly will facilitate the controllable synthesis and applications of carbon nanotubes.
2.2. Synthesis of MWCNTs
MWCNTs were discovered by Iijima in 1991 while vaporizing carbon in an electric arc  and were then produced at higher yield by increasing the pressure of the helium gas atmosphere . MWCNTs typically have inner diameters of ~3-20 nm and are then surrounded by concentric graphene sheets with an interstitial spacing between the sheets of ~3.4 Å. The number of concentric graphene sheets can range from 2 to ~100. High resolution TEM images of MWCNTs are provided in Fig. 3 . In Fig. 3a the high-resolution TEM image clearly shows that the distance between layers of the MWCNTs measures ~3.4 Å. Fig. 3b depicts a MWCNT with ~20 concentric shells. MWCNTs have electronic properties similar to those of graphite and are thus semimetals. They are promising for multiple applications including strong composite materials, ﬁeld emission displays, and adsorbents for gas separation or storage [40-47].
Similar to SWCNTs, a continuous low-cost production method producing MWCNTs that are easily puriﬁed is required for MWCNTs to be incorporated in emerging technologies. In 1997  and 1998 , ferrocene was utilized as a gas-phase catalyst in a CVD process for continuous MWCNT formation from methane at 1150 °C. However, the 1997 study reported materials containing more amorphous carbon than arc-generated MWCNTs, presumably due to a lower synthesis temperature than that achieved in the arc process . In the 1998 study, the outer layers of the tubes were not graphitic , making them more difﬁcult to purify. Later, ferrocene and ethylene were employed in CVD of MWCNTs between 650 and 950 °C . Again, carbon impurities were observed at high-density. The authors concluded that further work was necessary to improve the nanotube microstructure and yield . High-purity aligned, graphitic MWCNTs were synthesized via decomposition of a ferrocene-xylene mixture at ~675 °C. However, although the catalyst was supplied in the gas-phase, nucleation of tube growth occurred only for iron species deposited on a quartz substrate, resulting in a surface growth mechanism and limiting yields to available surface area . CVD techniques employing benzene pyrolosis  and the decomposition of ethylene  and acetylene  on supported metal catalysts have been demonstrated as viable large-scale production methods. MWCNTs have also been grown on supported metal particles or ﬁlms via CVD [55-59], plasma-enhanced CVD [60-70], hot-wire chemical vapor deposition [71,72], and plasma-enhanced HWCVD methods [73,74]. One HWCVD report employed evaporation of the Fe-Cr ﬁlament to supply a gas-phase catalyst, resulting in MWCNTs with a high density of structural defects and signiﬁcant carbon impurities . Although more research was deemed necessary, this method had potential for large-scale production, since it was not substrate dependent. In 2003, the ﬁrst continuous high-density MWCNT formation with minimal non-nanotube carbon impurites was demonstrated with HWCVD employing methane as the carbon source and ferrocene as a gas-phase catalyst . The metal catalyst impurities were simply removed via reﬂuxing in dilute HNO3 . Surprisingly, Multi-walled carbon nanotubes has been synthesized using acetylene as carbon sources with a metal-free mild chemical vapor deposition process by Du et al. . The authors not only gave a simple and facile way to synthesize MWCNTs without metal but also provided valuable information for a deeper understanding of CNT formation in CVD.
3. Synthesis of CNTs/metal oxide heterostructures
The transition metal oxides are an important family of inorganic nanomaterials with abundant properties in optics, electronics, magnetics and catalysis. The property of metal oxide nanomaterials can be further tuned by varying their composition, structure and morphology .
Composite materials based on CNTs and metal oxide nanomaterials integrate the unique characters and functions of the two types of components and may also exhibit some new properties caused by the cooperative effects between the two kinds of materials [78–82]. Therefore, these composite materials have shown very attractive potential applications in many ﬁelds. This section summarizes the handling of CNTs and the preparation of CNT-based nanocomposites.
3.1. Puriﬁcation and dispersion of CNTs
Generally, the carbon nanotubes as-prepared are grown as mixtures of carbon nanotubes and impurities such as amorphous carbon, metal catalyst particles and carbon nanoparticles. These impurities signiﬁcantly inﬂuence the properties of CNTs and limit their applications. Consequently, development of economical puriﬁcation methods has become an important issue to the development and practical applications of the CNTs. A commonly used puriﬁcation approach consists of two steps. The thermal or acid oxidation treatment on raw CNTs can effectively remove the amorphous carbon, carbon nanoparticles and carbon layers coated on the metal particles [83,84]. The following acid reﬂuxing treatment removes the residual naked metal-oxide particles . This method is time consuming and has the disadvantage of low yield and damaging the nanotubes. Some extraordinary methods such as magnetic ﬁltration, microwave irradiation, electrochemical oxidation, surfactant-assisted puriﬁcation and C2H2F4 or SF6 treatment have shown higher efﬁciency in removing the contaminants in the CNT samples and are less damaging to the nanotube structure [86–89].
Due to the strong - stacking interactions between the neighboring CNTs, they tend to aggregate into bundles, making it very difﬁcult for them to be dispersed in water and organic solvents. Their insolubility has become a great obstacle to the manipulation and application of CNTs. Dispersing nanotubes at the individual nanotube level is critical for a better performance of CNTs in most applications, especially the preparation of CNT-based composites. Therefore, many strategies have been explored to improve the solubility of CNTs in solvents. They can be classiﬁed mainly into two types, one is the sidewall covalent functionalization, and the other is the noncovalent modiﬁcation using guest molecules as solubilizers. By sonication in mixtures of sulfuric and nitric acids or sulfuric acid and hydrogen peroxide, carbonyl and carboxylic groups can be introduced onto the nanotubes . This is one of the most prevalently used covalent modiﬁcation methods. The modiﬁed CNTs can be further functionalized by esteriﬁcation or amidation reaction [91,92]. Other methods such as carbene cycloaddition, diazonium reaction and grafting of polymers have also been successfully used in the functionalization of CNTs [93,94]. The covalent methods convert the carbon atom hybridization from sp2 to sp3, leading to a disruption of electronic structure of CNTs. The noncovalent modiﬁcation methods, such as polymer and DNA wrapping, - stacking interactions with aromatic molecules and surfactant-assisted dispersion, are based on van der Waals or - stacking between CNTs and solubilizer molecules [95–98]. The noncovalent strategy offers the advantage of remarkably improving the CNTs’ solubility without disrupting the electronic structure of the tubes. Therefore it is more attractive than the covalent method for the maintenance of pristine structure and properties of CNTs. SWCNTs can be directly dispersed in the imidazolium-based ionic liquids simply by mechanical milling. The concentration of SWCNTs can be as high as 1wt%, which is remarkably higher than that of conventional covalent and noncovalent approaches . The prosperities of SWCNTs are well preserved, since only weak van der Waals force exists between SWCNTs and ionic liquids [100,101]. Therefore, imidazolium-based ionic liquids are superior solvents for the handling of CNTs [100,101].
3.2. Filling CNTs
The earliest attempt toward CNT-inorganic hybrids (in 1993) was the ﬁlling of MWCNTs with metal oxides (PbO  and Bi2O5 ). Because of their larger inner diameter (5-50 nm) compared with SWCNTs (1-1.5 nm), most efforts had been spent on ﬁlling MWCNTs, and it was not until ﬁve years later that Sloan et al. reported the ﬁlling of SWCNTs with RuCl3 . Recently, a few of researchers reported that magnetic nanoparticles or nanowires, such as cobalt, iorn and corresponding oxides, filled carbon nanotubes by various technologies and their properties were investigated as well [105-107]. However, carbon nanotube is difficult to be filled fully without few impurities duo to capillarity of itself.
Initially, the motivation arose mainly from the prospect of forming encapsulated or (upon oxidation) freestanding inorganic nanowires with new crystal structures or novel properties. Although both MWCNTs and SWCNTs have been ﬁlled with a vast number of compounds, little is known about their properties and potential in applications. This has been frequently blamed on high impurity levels in the synthesized hybrids, the lack of bulk quantities, and the need for speciﬁcally designed measurement devices . In general, the distinction should be made between the intrinsic properties of the ﬁller, the altered properties of the encapsulated material due to the conﬁned-space, and novel properties arising from interactions between the ﬁller and CNTs.
3.3. Ex situ approach: attaching metal oxide nanoparticles to CNTs
In this ex situ or building block approach, metal oxide nanoparticles are attached to the CNTs via linking agents that utilize covalent, π-π Stacking, or electrostatic interactions. In this approach, either the metal oxide nanoparticles or the CNTs (or the both) require modiﬁcation with functional groups. The type of functionalization and, thus, the strength of interaction determine the distribution and concentration of the metal oxide nanoparticles on the CNT surface.
3.3.1. Covalent Interactions
Carboxyl groups on the surface of acid-treated CNTs are often used to attach amine-terminated or mercapto-terminated metal oxide nanoparticles via amide bonds . This can be achieved either by directly linking amine-terminated or mercapto-terminated nanoparticles with the carboxyl groups or by modifying these carboxyl groups into thiol groups, which then anchor to colloidal nanoparticles. In a similar way, QDs have been linked by ﬁrst stabilizing them with a mixed monolayer of trioctylphosphine oxide (TOPO) and 2-aminoethanethiol . The resulting amino-functionalized QDs then reacted with the carboxylic groups of the acid-treated CNTs to form amide bonds.
Metal oxides can be attached to the carboxyl groups without any linking agent due to their hydrophilic nature, as recently demonstrated for MnO2 , MgO , and TiO2 . However, the authors observed only weak interactions between the oxides and the acid-terminated CNTs, resulting in rather nonuniform distributions of the nanoparticles. Better adhesion was observed when capping agents were used. For instance, Sainsbury and Fitzmaurice produced capped TiO2 via a standard sol-gel process using titanium tetraisopropoxide (TTIP) as precursors with cetyltrimethyl ammoniumbromide (CTAB) as the capping agent . MWCNTs were modiﬁed with 2-amino-ethylphosphoric acid and then mixed with the oxide nanoparticles. The authors showed that the phosphonic acid groups on the CNTs were well-distributed and provided an excellent driving force for the attachment of TiO2 nanoparticles (Fig. 4).
3.3.2. π-π stacking
This approach uses the moderately strong interactions between delocalized π-electrons of CNTs and those in aromatic organic compounds, such as derivatives of pyrene [115-117], porphyrins [118-120], phthalocyanines , or combinations thereof , as well as benzyl alcohol or triphenylphosphine (Fig. 5) . These molecules are often modiﬁed with long alkyl chains that are terminated with thiol, amine, or acid groups, which can then connect to metal oxide nanoparticles and enable their attachment to pristine CNTs via π-π stacking. For example, Li et al. used pyrene derivatives with a carboxylic termination to anchor magnetic nanoparticles such as Co or Fe3O4 .
One of the major advantages of this approach is that the pyrene compounds remain strongly adsorbed on the CNT surface after workup steps (e.g., washing, ﬁltration) and thus provide enhanced solubility and allow continuous redispersing of the modiﬁed CNTs in various aqueous and organic solvents. Furthermore, spectroscopic experiments on CNT/Pt  and CNT/porphyrin hybrids[118,126] revealed an enhanced charge transfer from inorganic nanoparticles to the CNTs, mediated by the aromatic compound. This was also observed for attached Co and Fe3O4 nanoparticles , whose magnetic and electronic properties were altered due to a strong electron transfer. Moreover, this effect is tunable by the length of the chain.
3.3.3. Electrostatic interactions
The approach utilizes electrostatic interactions between modiﬁed CNTs and metal oxide nanoparticles. Among the known examples, the deposition of ionic polyelectrolytes to attract charged nanoparticles is the most common route [127-131]. These polyelectrolytes typically bond covalently to the functional groups on the CNT, in contrast to polyethyleneimine (PEI), which interacts with CNTs via physisorption . For instance, Sun et al. deposited Al2O3, ZrO2, and TiO2 nanoparticles on charged CNTs in a slightly modiﬁed way . CNTs were pretreated in NH3 at 600 °C to induce a positive surface charge. The addition of PEI increased the positive charges even further and enabled a better dispersion. Commercially available α-Al2O3 and 3Y-TZP were then dispersed in poly(acrylic acid) (PAA), which provided a negative surface potential over a wide range of pH values. Upon mixing, the Al2O3 and ZrO2 nanoparticles formed strong electrostatic attractive interactions and covered the CNT surface completely.
Sun et al. attached nanocrystals of TiO2 to acid-treated SWCNTs, also using PEI as a modiﬁer (Fig. 6) . In the ﬁrst step, TiCl4 was mixed with PEI, whose charged amino groups were protonated at a pH of 8. The positively charged amino groups of PEI accelerated the hydrolysis of TiCl4 into TiO2-nanoparticles and stabilized them electrosterically. These amine-terminated TiO2-nanoparticles with positive charge then attached to acid-treated SWCNTs, either via amide linkage or through electrostatic interaction. Another route has been suggested by Jerome et al. , who grafted MWCNTs with poly-2-vinylpyridine (P2VP) to form carboxylate terminated alkyl chains, onto which positively charged magnetic Fe3O4 nanoparticles were anchored. The main advantage of the polymer route is that the polymers provide a very dense, uniform distribution of either negative or positive charges over the entire CNT surface, which enables very dense assemblies of metal oxide nanoparticles.
In summary, these few examples demonstrate the simplicity and feasibility of the ex situ approach, which remains the method of choice for the deposition of metal oxide nanoparticles. The main advantage is the possibility of using prepared nanoparticles with controlled morphology, structure, shape, and size, and, therefore, a good structure property relationship. The downside of this route, however, is the need to chemically modify either the CNTs or the metal oxide. This process is often work-intensive, and functionalization alters both the surface chemistry of the CNTs and also, particularly for SWCNTs, their physical properties. Furthermore, the use of predeﬁned building blocks restricts the synthesis of novel hybrid materials and, thus, the development of new physical properties.
3.4. In situ synthesis directly on the CNT surface
The metal oxides or hydroxides can also be formed directly on the surface of pristine or modiﬁed CNTs. The main advantage of this route is that the metal oxide or hydroxide can be deposited as a continuous amorphous or single-crystalline ﬁlm with controlled thickness, or as discrete units in the form of nanoparticles, nanorods, or nanobeads. Furthermore, the CNTs may act as a support to stabilize uncommon or even novel crystal phases or prevent crystal growth during crystallization and phase-transformation processes. Finally, a variety of chemical and physical synthesis techniques can be applied. The deposition can be carried out either in solution via electrochemical reduction of metal salts, electro- or electroless deposition, sol-gel processing, and hydrothermal treatment with supercritical solvents, or from the gas phase using chemical deposition (CVD or ALD) or physical deposition (laser ablation, electron beam deposition, thermal evaporation, or sputtering).
3.4.1. Electrochemical techniques
Electrochemistry is a powerful technique for the deposition of various metal oxide nanoparticles, as it enables effective control over nucleation and growth [136,137]. Most research has been conducted on the deposition of metal oxides, as they are the metal oxides of choice for applications like heterogeneous electrocatalyst, sensors, supercapacitors and so on. In general, metal oxide nanoparticles are obtained via reduction of metal complexes by chemical agents (chemical reduction), or by electrons (electrodeposition). The size of the metal oxide nanoparticles and their coverage on the sidewalls of CNTs can be controlled by the concentration of the metal salt and various electrochemical deposition parameters, including nucleation potential and deposition time .
188.8.131.52. Chemical reduction and oxidation
These techniques involve reactions, in which the reduction of the precursor is carried out with liquid or gaseous reducing agents with the aid of heat, light, ultrasound, microwave, or supercritical CO2 [139,140]. As an example, Sivvakkumar et al. deposited MnO2 via chemical reduction of KMnO4 . The authors suspended the CNTs in Na-p-toluene sulfonate and pyrrole, which polymerized with the aid of ultrasonication. KMnO4 was then slowly added and reduced with acetonitrile to form hydrous MnO2. A very elegant variation of this process is shown in Fig. 7 and uses KMnO4 as both the oxidizer and reactant . In detail, pristine MWCNTs were ﬁrst oxidized under reﬂux with KMnO4, which introduced exclusively hydroxyl groups on the sidewalls of CNTs, in contrast to other oxidation treatments, e.g., with oxidizing acids. These hydroxyl groups then acted as anchors for Mn7+ ions, which subsequently were reduced to Mn4+ with citric acid to form a coating of -MnO2. For comparison, a pretreatment of the CNTs in strong acids, which induces the formation of carboxyl groups, resulted instead in γ-MnO2 . Therefore, this work provides an interesting example of the effect of the CNT surface chemistry on the crystal structure of the metal oxide coating. In contrast to MnO2, the deposition of other metal oxides typically requires oxidizing rather than reducing processes. For instance, Huang et al. added acid-treated CNTs to a solution containing ammonium metavanadate . The adsorbed VO2+ ions were then oxidized with oxalic acid to V2O5. A different approach combined the reduction of cationic precursors by hydrogen with a water-in-oil microemulsion technique for the deposition of metal oxide nanoparticles . Sun et al. used a slightly modiﬁed process . The CNTs was mixed ﬁrst with an aqueous solution of sodium dodecylbenzene sulfonate (NaD-DBS) and then with a mixture of Triton-X and cyclohexane, which resulted in very small water droplets on the CNT surface. Upon adding zinc acetate as the metal precursor, the Zn2+ ions concentrated in the aqueous phase and then reacted with NH3 or LiOH to form spherical, hollow ZnOH nanoparticles. Subsequent calcinations oxidized them to create small and dense ZnO nanoparticles. In all cases, the microemulsion technique produced ﬁne dispersions of small nanoparticles.
Many of the above-mentioned reduction/oxidation techniques are very time-consuming and as such allow impurities in the bath solution to be incorporated into the inorganic phase. In contrast, electrodeposited nanoparticles, exhibit higher purities as well as a good adhesion to the CNT surface .
In most cases, simple van der Waals interactions between the CNTs and the metal oxide nanoparticles seem to be sufﬁcient to provide strong enough adhesion. Although most research currently concentrates on the electrodeposition of metal nanoparticles, there have also been a few reports on electrodeposited metal oxides. As an example, TiCl3 was used as a precursor and electrolyte and was kept at pH 2.5 with HCl/Na2CO3. The deposition was then carried out via galvanostatic oxidation with 1 mA/cm2 and resulted in a rather irregular and partial coating of a mixture of anatase and TiO2-B . The galvanostatic approach (3 mA/cm2) has also been applied to codeposit Ni and Co oxides from their nitrates, with Pt and saturated calomel as the counter electrodes and reference electrodes, respectively . This was also demonstrated by Kim et al., who produced a continuous 3 nm thick coating of RuO2 via the potential cycling method while varying the potential from 200 to 1000 mV with a scan rate of 50 mV/s . They observed that the gas atmosphere during the postannealing process had a signiﬁcant effect on the morphology of RuOx .
One advantage of this technique is that the electrodeposition occurs to the same extent on both the sidewalls of the tubes and the tips . Consequently, the presence of carboxyl or hydroxyl groups as activators is not required. However, the major drawback of electrodeposition is that it is difﬁcult to produce bulk quantities.
3.4.2. Sol-gel process
The sol-gel process is a versatile, solution-based process for producing various ceramic and glass materials in the form of nanoparticles, thin-ﬁlm coatings, ﬁbers, or aerogels and involves the transition of a liquid, colloidal “sol” into a solid “gel” phase . The sol-gel process is a cheap and low-temperature technique that allows ﬁne control of chemical composition and the introduction of lowest concentrations of ﬁnely dispersed dopants. One of the major drawbacks is that the product typically consists of an amorphous phase rather than deﬁned crystals and, thus, requires crystallization and postannealing steps.
In general, the sol-gel process has emerged as the most common technique to synthesize CNT/metal oxide hybrids. Early attempts concentrated on the dispersion of CNTs within a matrix of metal oxide nanoparticles. Vincent et al. synthesized TiO2 nanoparticles using metal organic precursors and acetic acid as a gelator . They observed that the dispersion of pristine CNTs was more stable when the TiO2 nanoparticles had been produced in the presence of the CNTs (in situ) compared with the simple mixing of the two materials. Upon reducing the amount of TiO2 with respect to CNTs, Jitianu et al. obtained a thin but rather irregular and partial coating of TiO2 on CNTs [154,155]. Typically, the thickness of the coating can be controlled by various parameters, such as the reaction time , the reaction composition, and the choice of metal precursor . For instance, in the case of TiO2, the use of titanium tetraisopropoxide (TTIP) produced irregular coatings [154,158], while tetraethoxy orthotitanate (TEOT)  or tetrabutoxy orthotitanate (TBOT) [157,159] enabled a more uniform deposition. The sol-gel process was sometimes carried out under reﬂux , or with the aid of ultrasonication , microwave , or magnetic agitation , in order to enable faster and simultaneous nucleation resulting in a more homogeneous coating.
These early works used pristine CNTs, whose hydrophobic nature provides little attractive interaction with the metal oxide and thus limits the quality of the coating. Similar to the ex situ approach, the most common approach to change the surface chemistry of CNTs is to treat them in strong oxidizing acids (H2SO4/HNO3). This process introduces a variety of organic groups, with limited control over their number, type, and location, and causes surface etching and shortening of the tubes. Consequently, the metal oxide coatings on acid-treated CNTs were often nonuniform, although they provided better interaction in comparison with pristine CNTs. Despite these drawbacks, most researchers have used such acid-treated CNTs for various metal oxide coatings, including SnO2 [160,161,163-165], TiO2 [159,166-168], RuO2 [169,170], CeO2 , NiO , and mixed oxides .
In a similar way to the ex situ approach, noncovalent attractions and π-π interactions can be used to grow the metal oxide on the surface of CNTs. Cao et al. modiﬁed CNTs with surfactants such as sodium dodecylsulfate (SDS) . The hydrophobic aliphatic chain interacted with the surface of the CNTs, while the hydrophilic end attracted the metal ions of the RuCl3 precursor, which then reacted to form RuO2. Recently, this author has developed a nondestructive, simple process to coat pristine CNTs with TiO2 by using benzyl alcohol as a surfactant . Benzyl alcohol adsorbs onto the CNTs’ surface via π-π interactions with the alcohol’s benzene ring, while simultaneously providing hydrophilic hydroxyl groups for the hydrolysis of the titanium precursor (TBOT) (Fig. 8). In contrast to the sample without benzyl alcohol (Fig. 8A), the addition of small amounts of benzyl alcohol resulted in a very uniform coating that covered the whole CNT surface. The work further showed that benzyl alcohol strongly affected the phase transition from anatase to rutile, providing very small and uniform rutile nanocrystals with very high speciﬁc surface areas (60-100 m2/g) without too great a hindrance of the anatase to rutile transformation.
In contrast to the ex situ approach, the use of electrostatic interactions for the in situ sol-gel route has been demonstrated for a few metal oxides. As an example, Hernadi et al. used CNTs that had been pretreated with SDS, dried, and redispersed in 2-propanol . Using metal halides as precursors, the authors could successfully produce coatings of Al2O3 and TiO2. Vietmeyer et al. used acid-treated CNTs to attract Zn2+ ions (using zinc acetate), which then reacted with LiOH in an ice-water bath to form ZnO nanoparticles . While some metal oxide nanoparticles were attached to the CNT surface and tips, most of the nanoparticles formed large clusters rather than a continuous coating. For comparison, Jiang et al. enhanced the negative charge on the surface of acid-treated CNTs by simply depositing a thin layer of SDS and carried out the same reaction with zinc acetate and LiOH . This surface modiﬁcation signiﬁcantly enhanced the attractive interactions with the metal ions and led to a more uniform coating with ZnO crystals.
3.4.3. Hydrothermal and aerosol techniques
In recent years, many organic-inorganic hybrids have been produced by hydrothermal techniques . In contrast to standard sol-gel routes, the hydrothermal method typically enables the formation of crystalline particles or ﬁlms without the need for postannealing and calcinations. Furthermore, the forced crystallization enables the formation of metal oxide nanowires and nanorods .
184.108.40.206. Vapor-assisted, polyol-assisted process
In this simplest case of hydrothermal synthesis, pristine or acid-treated CNTs were added to an aqueous solution of the precursor and treated in an autoclave at temperatures between 100 and 240 °C to produce crystalline ﬁlms of ZnO , TiO2 , or Fe2O3 . These works consistently produced dense coatings of spherical or slightly elongated nanoparticles. Zhang et al. used aligned CNTs, which they precoated with a thin, amorphous layer of ZnO via magnetron sputtering . Then they dissolved a ﬁne ZnO powder in NaOH at a pH of 10-12, which provided a saturated solution of Zn(OH)42-. The modiﬁed CNT carpet was then placed top-down in an autoclave, ﬂoating on the precursor solution. By keeping the reaction at a temperature of 100 °C for several hours, the Zn precursor nucleated on the CNT-ZnO ﬁlm to grow ZnO nanowires perpendicular to the CNTs, with a thickness of 30-70 nm and lengths of up to 0.5 µm (Fig. 9).
In general, speciﬁc molecules provide efﬁcient control of the crystal size of the nanoparticles, which hinder the crystal growth by steric conﬁguration (capping agents). For example, Yu et al. dissolved copper acetate in water and diethylene glycol and added acid-treated CNTs [184,185]. Upon heating in an autoclave at 180 °C, the diethylene glycol-capped copper species condensed to CuOx and nucleated to form small Cu2O crystals. After a reaction time of 2 h, the crystals were 5-10 nm in diameter and covered by an amorphous layer. Similarly, small crystals of Fe3O4 were produced by Jia et al., who used polyethylene glycol (PEG) and FeCl3 and a reaction temperature of 200 °C . However, the 5 nm crystals agglomerated to about 180 nm aggregates (nanobeads), which attached preferably to the carboxyl groups on the surface of acid-treated CNTs. Consequently, the magnetite nanobeads were concentrated at the tips of the CNTs and acted as a glue to form heterojunctions between the CNTs (Fig. 10).
220.127.116.11. Supercritical solvent
A very important hydrothermal method involves the use of supercritical CO2 as an antisolvent that reduces the solvent strength of ethanol, resulting in the precipitation of the oxide due to high saturation. Using metal nitrates or halides, this method has been applied to deposit Eu2O3 , CeO2 , La2O3 , Al2O3 , SnO2 [189,190], and Fe2O3  onto pristine CNTs. Sun et al. used supercritical ethylenediamine as a solvent to produce thin coatings of RuO2 . They also observed various morphologies and structures of cerium oxide by simply changing the reaction temperature . For instance, the authors could alter the composition of cerium oxide from preferentially Ce2O3 at 120 °C to CeO2 at 150 °C. In contrast, a reaction temperature of 120 °C was needed to obtain a coating of SnO2, while at 35 °C the oxide was only encapsulated .
3.4.4. Gas-phase deposition
Chemical and physical vapor deposition techniques are among the most common methods to produce metal oxide nanomaterials, as they provide excellent control over the size, shape, and uniformity of the oxide material. Furthermore, it is possible to deposit thin, continuous ﬁlms on carbon substrates, without altering the 3D integrity of vertically aligned CNTs. This section provides examples of the synthesis of various CNT/metal oxide hybrids using physical techniques, such as evaporation, sputtering, and pulsed laser deposition (PLD), and chemical methods, including chemical vapor deposition (CVD) and atomic layer deposition (ALD).
18.104.22.168. Evaporation and sputtering
Physical vapor deposition involves the evaporation of material in a crucible under high vacuum, using either resistive heating (thermal evaporation) or electron bombardment (electron beam deposition). In contrast, sputtering (magnetron and radio frequency, RF) relies on plasma (typically argon) to bombard the target material, which can be kept at a relatively low temperature. Reactive sputtering involves a small amount of oxygen, which reacts with the sputtered material to deposit oxides. The deposition of metal oxides via thermal evaporation has been demonstrated by Kim et al., who mixed annealed CNTs with Zn powder in a ratio of 1:12 . Depending on the reaction temperature, the Zn particles reacted with oxygen impurities in argon to form a coating on the CNTs consisting either of spherical particles (450 °C), nanowires (800 °C), or short nanorods (900 °C). RF or magnetron sputtering has been used to deposit RuOx,  and ZnO . Furthermore, Jin et al. have cosputtered Ba and Sr in an oxygen atmosphere to obtain a BaO/SrO coating . In most of these works, the coating around the CNTs was generally conformal, although in the case of vertically aligned CNTs (“carpet”), the metal oxide material was deposited predominantly along the top of the carpet. Interestingly, Fang et al. observed that the distribution of RuO2 particles on vertically aligned CNTs was signiﬁcantly better on nitrogen-doped CNTs compared with pure CNTs . It is well-known that the incorporation of nitrogen into the sp2-type walls of CNTs causes many structural defects (pyridine-like bonding) due to the different valence of nitrogen ions. It seems that these defects are more reactive toward the adsorption of RuO2 than the graphitic walls of pure CNTs and allow a uniform dispersion along the sidewalls of nitrogen-doped CNTs (Fig. 11).
In summary, sputtered ﬁlms typically have a better adhesion to the substrate than evaporated ﬁlms and a composition closer to that of the source material. Sputtering also enables the deposition of materials with very high melting points and can be performed “top-down”, while evaporation must be operated “bottom-up”. On the other hand, evaporation techniques typically offer better structural and morphological control and more ﬂexible deposition rates.
22.214.171.124. Pulsed laser deposition
Pulsed laser deposition (PLD) is related to the evaporation techniques but utilizes a high-power pulsed laser beam. The directed laser pulse is absorbed by the target, vaporizes the material, and creates a plasma plume containing various energetic species, such as atoms, molecules, electrons, ions, clusters, particulates, and molten globules, which then expand into the vacuum and deposit on a typically hot substrate to nucleate and grow as a thin ﬁlm. This process can occur in ultrahigh vacuum or in the presence of a background gas, such as oxygen, which is commonly used when depositing oxides. Ikuno et al. used individual MWCNTs (grown by arc discharge), which were attached to a molybdenum plate via electrophoresis. A pulsed Nd:YAG (yttrium aluminum garnet) laser with a wavelength of 355 nm was focused onto a target at a repetition rate of 10 Hz. A single-crystalline Si wafer and pellets of Zr, Hf, Al, ZnO, Au, and Ti were used as targets for the coating of SiOx, ZrOx, HfOx, AlOx, and ZnOx [198,199]. The advantages of this technique over other thin-ﬁlm deposition methods include the relatively simple basic setup and the operation at room temperature. On the other hand, PLD has a lower average deposition rate than other deposition techniques, such as CVD or evaporation/sputtering techniques, but is faster than ALD.
126.96.36.199. Chemical vapor deposition
Chemical vapor deposition (CVD) is a versatile technique often used in the semiconductor industry that involves the growth of a solid material from the gas phase via chemical reaction at the surface of a substrate. In contrast to high-pressure/high-temperature synthesis, the CVD technique typically operates at medium temperatures (600-800 °C) and at slightly reduced atmospheric pressures. Because CVD utilizes reagents of very high purity, the technique is capable of synthesizing crystals with controlled purity and composition. Other advantages of CVD include the high deposition rate, good degree of control (purity and composition), and easy scalability. However, due to the fast deposition, it is difﬁcult to achieve uniform and defect-free coatings when scaling down to a few nanometers. Several groups have used CVD to synthesize CNT-metal oxide hybrids with SnO2  and RuO2 . Kuang et al. deposited acid-treated MWCNTs on a Si waver and heated them to 550 °C in a SnH4-containing N2 atmosphere . At this temperature, the precursor decomposed, attached to the functional groups of the CNTs, and reacted with the oxygen impurities to produce SnO2. In a similar way, CNTs/RuO2 , CNTs/Co3O4  and CNTs/ZnO [203-205] have been synthesized by directly coating of prepared CNTs. On the other hand, An example of the in situ growth of CNTs is the work of Liu et al., who used a water-assisted CVD process to produce CNTs with a ZnO coating . Most of the ZnO coating was observed at the tip of the CNTs. An interesting alternative to ZnO was demonstrated by Ho et al. . The authors used Ni catalyst particles, supported on MgO, which were deposited on a Si wafer and placed inside a tube furnace. ZnO powder was put inside a thin ceramic tube, whose ends were covered with Al foil, and placed inside the reactor tube, close to the catalyst powder. Upon reaching a certain temperature (300-350 °C), assisted via a plasma-enhanced CVD technique, CNTs began to grow on the Ni particles and kept growing as the temperature was steadily increased to 700 °C over a period of about 6-7min. At this temperature, the Al foil melted and exposed the ZnO powder, which was instantaneously transformed to Zn vapor via carbothermal reduction and deposited on the still-growing CNTs as a thin coating of ZnO.
188.8.131.52. Atomic layer deposition
In contrast to CVD, the precursors for atomic layer deposition (ALD) are kept separate and exposed sequentially. Ideally, each precursor forms a monolayer on the substrate, and the excess vapor is removed before the next precursor is introduced. This process is then repeated until the deposited ﬁlm reaches the desired thickness. Hence, ALD ﬁlm growth is self-limiting and based on surface reactions, which enables deposition control on the atomic scale. As an example, Gomathi et al. used metal chloride precursors to coat acid-treated MWCNTs with TiO2 and Al2O3 . Similarly, Javey et al. demonstrated coatings of ZrO2 as thin as 8 nm covering the top of horizontally attached SWCNTs for device applications . ALD has unique advantages over other thin-ﬁlm deposition techniques, as it can be operated at low temperatures and allows exact control over the thickness of the deposited coating. However, because of the sequential exposure of the precursors, the technique has the lowest deposition rate compared with CVD and PLD.
4. Properties and potential applications of CNTs/metal oxide hybrids
The improved performances of CNT/metal oxide hybrids are demonstrated in many applications, such as photocatalysis, electrocatalysis, and environmental catalysis, gas sensors and chemical sensors, supercapacitors and batteries, and ﬁeld emission devices. In the section, some applications of electrocatalysis, electrochemical sensors, supercapacitors and batteries are highlighted and summarized as follow.
Electrocatalyst is a new catalyst depending on electric energy. Which accelerate the reactions on the interface between electrode and electrolyte. It has significance in research work and also has important application value on organic wastewater treatment and degradation, electrolytic desulfurization, and electroreduction study. As an electrocatalyst, two basic conditions are necessary: (a) electrical conductivity and transfer free electron well; (b) efficient catalytic activity towards target substrate. Metal, especially noble metal, and some metal oxide or hydroxide are widely used as electrocatalysts . In contrast, some common transition metal oxides or hydroxides, such as TiO2, SnO2, Ni(OH)2, have many advantages including low cost, facile preparation, and thus are more interesting for wide study. CNTs endows CNT/metal oxide or hydroxide composites enhancement on electrocatalysis duo to electric conductivity and fast electron transfer.
For example, Qiao et al. reported that the MWCNTs/Ni(OH)2–Ni electrode showed better catalytic effect on the oxidation of CH4 in 1.0 M NaOH than Ni(OH)2–Ni electrode . ZnO-NWs/MWCNTs nanocomposite had been prepared via a hydrothermal process by Mo et al., and showed remarkable electrocatalytic activity towards H2O2 by comparing with bare MWCNTs . Subseguently, Ma et al. discovered that ZnO-MWCNTs/Naﬁon ﬁlm showed fast and excellent electrocatalytic activity to not only H2O2, also trichloroacetic acid . Other metal oxide or hydroxide, such as FeOOH  and cobalt-coordinated polypyrrole , have been reported have obvious electrocatalysis towards oxygen reduction reaction. Recently, we synthesized CNTs/nickel glycolate polymer core-shell heterostructures and found that the composite have significant electrocatalysis towards glucose in 0.5 M NaOH, and catalytic activity dependent obviously on the thickeness of the nickel glycolate polymer on MWCNTs (Fig. 12).
The role of CNTs is often attributed to their ability to stabilize highly dispersed catalyst nanoclusters, resulting in higher speciﬁc surface areas. So, There is also important significant for fuel cell and biosensor to study further electrocatalysis of CNTs/metal oxide or hydroxide composites.
4.2. Electrochemical sensors
Metal oxide semiconductors (MOS) are prominent examples of sensing materials in gas sensors, as their electrical properties are highly affected by the surrounding gas environment. For instance, tungsten trioxide (WO3) shows sensitivity to pollutants such as SO2, H2S, NO, and NH3 [216,217], while SnO2 is sensitive to NOx, CO, ethanol, and C2H4 . However, their sensing properties often suffer degradation due to growth and aggregation. In contrast with metal oxide sensors, CNTs exhibit excellent adsorption properties due to their high speciﬁc surface area, which provides a large number of active surface sites [219-221]. As the CNTs’ electric properties are effectively altered by very small amounts of adsorbed gas molecules, the CNT gas sensor can be operated at temperatures close to room temperature. However, as MWCNTs are not very sensitive to ambient gas, the use of CNTs as gas sensors is mainly restricted to SWCNTs. Furthermore, due to their long recovery times, CNT-based sensors typically need reactivation.
CNTs/MOS hybrid composite sensors have been fabricated and investigated widely. These sensors don’t noly improve the efficiency of the metal oxide based sensors, such as enhanced sensitivity and selectivity to target gases, reduced response and recovery times, but also are operated at lowered temperature, even room temperature. Similar to core/shell heterostructures like MOS/CdS, CNT/MOS hybrids have shown improved photoluminescent quantum efﬁciencies and enhanced gas-sensing properties including reduced response and recovery times [163,222]. So far, CNT/SnO2 has been tested for detection of CO , NO2 [201,203], NH3 , formaldehyde , and ethanol . Wei et al. used a sol-gel process to coat pristine SWCNTs with SnO2 and investigated the gas-sensing performance for NO2 at room temperature . They observed considerably enhanced sensitivities (∆R/∆C, Fig. 13) compared with the pure SnO2 sensor. Because the morphology and surface area of the hybrid sensors were similar to those of the pure SnO2, and the observed sensitivities increased with increasing CNT loading, the authors concluded that the advanced sensing behavior originated from a common interface with CNTs. In contrast to conventional SnO2 sensors, which typically operate at temperatures between 200 and 500 °C, the SWCNT/SnO2 hybrid gas sensors could indeed be operated at room temperature. When the NO2 gas molecules adsorb on the surface of pure SnO2, they extract electrons, leaving the oxide surface positively charged. This leads to the formation of a depletion zone and to an increase in the sensor resistance. In the CNT/SnO2 hybrid sensor, the electric properties of the oxide are strongly enhanced by the highly conducting CNTs. Consequently, the sensor resistance is dominated by the Schottky barrier at the interface between the n-type SnO2 grains and the p-type CNTs, causing the formation of additional depletion layers, which then ampliﬁes the increase in resistance upon NO2 adsorption and enables the operation of the gas sensor at room temperature.
As CNTs/metal oxide hybrid sensors emerges, some of which were investigated to applied in liquid sensing, especially biosensors including glucose sensor, hydrogen peroxide, hydrazine sensor and nitrite detection etc. The sensors have significant potential application in biology and medicine because of unavoidable drawbacks of enzyme sensor, such as temperature, PH, and unicity. More and more CNTs/metal oxide hybrids were reported to be used as various sensors in liquid.
For instance, Jiang et al. reported a highly sensitive nonenzymatic glucose sensor based on CuO nanoparticles-modiﬁed carbon nanotube electrode by sputtering deposition method . The CuO/MWCNTs electrode exhibits an enhanced electrocatalytic property, low-working potential, high sensitivity, excellent selectivity, good stability, and fast amperometric sensing towards oxidation of glucose, thus is promising for the future development of nonenzymatic glucose sensors. Glucose was also detected with CNT/Fe3O4 hybrids electrochemically doped glucose oxidase reported by Liu et al.  The PA–Fe3O4–CNT-based glucose sensor shows much higher sensitivity and linearity than the PA–Fe3O4-based sensor, indicating that CNTs signiﬁcantly enhance the performances of the biosensor. A novel hydrazine electrochemical sensor based on a carbon nanotube-wired ZnO nanoﬂower-modiﬁed electrode was reported via a simple process (ammonia-evaporation-induced synthetic method) by Fang et al. . The authors observed that an optimized limit of detection of 0.18 M at a signal-to-noise ratio of 3 and with a fast response time (within 3 s).
4.3. Supercapacitors and batteries
Reliable and affordable electricity storage is a prerequisite for optimizing the integration of renewable energy systems. Energy storage, therefore, has a pivotal role to play in the effort to combine a future, sustainable energy supply with the standards of technical services and products. For both stationary and transport applications, energy storage is of growing importance as it enables the smoothing of transient and/or intermittent loads and the downsizing of base-load capacity with substantial potential for energy and cost savings. The extended lifetime of batteries in handheld devices is credited not only to higher energy densities but also to a simultaneous reduction of energy consumption of the portable devices. In contrast, the electric vehicle has failed to become the accepted mode of transportation mainly because of the battery. Short distances between recharging and a limited service life of the battery are to blame, but also the incredible weight and volume of the batteries. Electrochemical capacitors (ECs) are energy-storage devices that possess higher energy and power density than conventional dielectric capacitors and batteries and are used in applications including electric vehicles, noninterruptible power supplies, dc power systems, lightweight electronic fuses, memory backups, and solar batteries . The challenges for these applications concern limitations in volumetric/gravimetric power densities and RC time, long life, safety, simplicity of design, cost, and the possibility of recharging, and can only be accomplished by specially designed materials.
According to the mechanism of energy storage, ECs can be categorized into two classes : (a) electrochemical double layer capacitors (EDLC), based on double-layer capacitance due to charge separation at the electrode/electrolyte interface, which thereby need materials with high speciﬁc surface area (e.g., activated carbon, CNTs), and (b) pseudocapacitors or supercapacitors, based on the pseudocapacitance of faradaic processes in active electrode materials such as transition metal oxides and conducting polymers.
Because of their exceptional electronic properties, which allow ballistic transport of electrons over long nanotube lengths, CNTs have been considered a most promising candidate for electrochemical capacitors [230,231]. However, pure CNTs possess a rather low speciﬁc capacitance, typically about 10-40 F/g, which depends on the microtexture, purity, and electrolyte . A considerable enhancement can be expected from the combination of CNTs with an electroactive material, which provides the additional pseudocapacitance while each tube acts as a minute electrode. the electrochemical stability of transition metal oxides makes them a better choice, provided they are highly conducting. A wide range of oxides has been investigated for use in CNT hybrids, including NiO [171,232,233], MnO2 [234-237], V2O5 [238,239], and RuO2 [169,192,194]. In all of these studies, the synergistic effects of CNT oxide hybrids have shown a considerable improvement of the otherwise poor electric properties and deﬁcient charge transfer channels of the pure oxide.
Among these transition metal oxides, ruthenium oxides are regarded as the most promising electrode material for supercapacitor applications due to their high speciﬁc capacitance, highly reversible redox reactions, wide potential window, and very long cycle life . Park et al. reported a speciﬁc capacitance for CNT/RuO2 (13 wt %) of 450 F/g at a potential scan rate of 20 mV s-1, which could be further enhanced, by using hydrous ruthenium oxide and functionalized CNTs, to 800 F/g . Reducing the thickness of the RuO2 layer to 3 nm led to an even higher capacitance (1170F/g at a potential scan rate of 10 mV s-1) . All of these studies also demonstrated longer lifetimes and greater stabilities and rate capabilities, while the speciﬁc capacitances were in general considerably higher than those observed for pure MWCNTs (<80 F/g) or pure RuO2 (<400 F/g).
In view of the rather high costs and environmental issues concerning RuO2, and despite the lower speciﬁc capacitances, there has been a clear trend toward the use of hydrous manganese oxides in the past few years. Xie et al. produced a CNT/MnO2 hybrid by in situ reduction of KMnO4 on MWCNTs with citric acid and observed that the speciﬁc capacitance increased from 18 to 190 F/g . Zhang et al. electrodeposited MnO2 “nanoﬂowers” onto the surface of vertical CNT arrays and obtained capacitances of about 200 F/g, as well as excellent rate capabilities (50.8%, capacity retention at 77 A/g) and a long cycle life (3% capacity loss after 20 000 charge/discharge cycles) . The authors proposed a model for the improved electrochemical storage characteristics based on high electronic conductivity in CNTs. In this model, the geometry of the MnO2 nanoﬂowers and their hierarchical localization at CNT junctions limits the diffusion length of ions within the MnO2 phase during the charge/discharge process and enhances the ionic conductivity of the hybrid.
To maximize the electrochemical utilization of the supercapacitor, it is desirable to (a) use a low loading of metal oxide and (b) increase the interfacial area between CNTs and metal oxide. Consequently, the preparation of a thin, uniform, connected coating on CNTs is expected to improve the speciﬁc capacitance signiﬁcantly. This was conﬁrmed by Nam et al., who observed increasing capacitances with decreasing NiO content and thus coating thickness .
A promising approach to enhance the capacitive performance has recently been reported by Sivakkumar et al., who synthesized a ternary hybrid of CNT/polypyrrole/hydrous MnO2, which showed a signiﬁcantly higher speciﬁc capacitance (280 F/g) compared to the binary CNT/MnO2 (150F/g) . The increase in capacitance is believed to be due to the better dispersion of hydrous MnO2 in the composite electrode. However, the presence of the polymer also accounts for the poor cyclability behavior. Fang et al. chose a different approach by depositing RuO2 on N-doped CNT , for which they measured considerably higher speciﬁc capacitances. The authors showed that the RuO2 particles were considerably better dispersed on N-doped CNTs than on pure CNTs, due to the presence of structural defects in N-CNTs. Consequently, the hybrids with N-doped CNTs had an enhanced interface, which resulted in their better performance as a supercapacitor (Fig. 14).
A good cyclability is crucial to a successful application as an anode material for lithium-ion batteries, as demonstrated by Chen et al. for CNT/SnOx hybrids . Pure CNTs typically show good cycle stability, but also a large and irreversible capacity loss in the ﬁrst cycle. The authors showed that well-dispersed SnOx on CNTs enhanced the electrochemical performance signiﬁcantly as the capacity fade of the hybrid electrode was strongly reduced compared to unsupported SnOx or pure CNT. The authors attributed the improvement in performance to the enhanced conductivity and ductility of the hybrid. This is in line with Zheng et al., who observed a 5-fold increase in electronic conductivity and thus enhanced cycling rate and stability in CNT/CuO hybrids compared to pure CuO.
In summary, electrochemical devices have been among the ﬁrst applications for which CNT/metal oxide hybrids were tested. In the long run, CNT hybrids are expected to strongly enhance the batteries’ intrinsic capacities, stabilities, and lifetimes, as well as the charging/discharging characteristics. Furthermore, the substitution of part of the heavy oxide material (e.g., in car batteries) with the lightweight CNTs will signiﬁcantly reduce the weight of the batteries.
5. Conclusion and future directions
As reviewed in the former publications, numerous synthetic methodologies have been developed for the preparation of CNTs and composites. In this chapter, besides the preparation of nanocomposites based on CNTs, we also focus on investigating the electrochemical applications CNT/metal oxide or hydroxide composites. There is a wealth of opportunities for nanoscale electrochemical devices based on carbon materials. Furthermore, when the electrode dimension approaches the double layer thickness, interesting and unusual kinetic and electrostatic effects occur. It is likely that carbon nanotubes electrodes will be key players in the investigation of such phenomena.
Financial support from Zhejiang Provincial Natural Science Foundation of China (Y4110304), Zhejiang Qianjiang Talent Project (2010R10025), the Educational Commission of Zhejiang Province of China (Z200909406) are gratefully acknowledged.
Li . Tang S. B. Lu L. Zeng H. C. 2007J. Am. Chem. Soc., 129, 9401
Iijima S. 1991Nature., 354, 56
Iijima S. 1993Nature., 363, 603
Harris P. J. F. 2003Carbon Nanotubes and Related Structures; Cambridge University Press: Cambridge, U.K.
Dillon A. C. Yudasaka M. Dresselhaus M. S. Nanosci J. 2004Nanotechnol., 407, 691
Avouris P. (2004 Bull M. R. S. 200
Jorio A. Dresselhaus G. Dresselhaus M. S. 2007Carbon Nanotubes: ad anced topics in sythesis, structure and properties; Springer: New York
Dillon A. C. Jones K. M. Bekkedahl T. A. Kiang C. H. Bethune D. S. Heben M. J. 1997Nature., 386, 377
Dillon A. C. Mahan A. H. Alleman J. L. Heben M. J. Parilla P. A. Jones K. M. Thin Solid. Films
Lehman J. H. Engtrakul C. Gennett T. Dillon A. C. 2005Appl. Opt., 44, 483
Lehman J. H. Deshpande R. Rice P. Dillon A. C. 2006IR Phys., 47, 246
Dillon A. C. Heben M. J. 2001Appl. Phys. A: Mater. Sci. Process., 72, 133
Dillon A. C. Mahan A. H. Deshpande R. Alleman J. L. Blackburn J. L. Parillia P. A. Heben M. J. Engtrakul C. Gilbert K. E. H. Jones K. M. To R. Lee S. H. Lehman J. H. 2006Thin Solid Films., 501, 216
Bethune D. S. Kiang C. H. Vries M. S. d. Gorman G. Savoy R. Vasquez J. Beyers R. 1993Nature., 363, 605
Lamy de la Chapells, S. Lefrant, P. Deniard, R. Lee, J. E. Fischer. ( Journet C. Maser W. K. Bernier P. Loiseau A. M. 1997Nature., 388, 756
Private Communication. Bandow S.
Guo T. Nikolaev P. Thess A. Colbert D. T. Smalley R. E. Chem Phys. Lett 1995
Thess A. Lee R. Nikolaev P. Dai H. Pitit P. Robert J. Xu C. Lee Y. H. Kim S. G. Rinzler A. G. Colbert D. T. Scuseria G. E. Tomanek D. Fischer J. E. Smalley R. E. 1996Science., 273, 483
Heben M. J. Dillon A. C. Gilbert K. E. H. Parilla P. A. Gennett T. Alleman J. L. Hornyak G. L. Jones K. M. 2002Hydrogen Mater. Vac. Syst., 671, 77
Dillon A. C. Parilla P. A. Alleman J. L. Gennett T. Jones K. M. Heben M. J. 2005Chem. Phys. Lett., 401, 522
Kataura H. Maniwa Y. Abe M. Fujiwara A. Kodama T. Kikuchi K. Imahori H. Misaki Y. Suzuki S. Achiba Y. 2002Appl. Phys. A: Mater. Sci. Process., 74, 349
Dillon A. C. Gennett T. Jones K. M. Alleman J. L. Parilla P. A. Heben M. J. 1999Adv. Mater., 11, 1354
Dai H. Rinzler A. G. Nikolaev P. Thess A. Colbert D. T. Smalley R. E. 1996Chem. Phys. Lett., 260, 471
Peigney A. Laurent C. Dobigeon F. Rousset A. J. 1997Mater. Res., 12, 613
Hafner J. H. Bronikowski M. J. Azamian B. R. Nikolev P. Rinzler A. G. Colbert D. T. Smith K. A. Smalley R. E. 1998Chem. Phys. Lett., 296, 195
Cheng H. M. Li F. Su G. Pan H. Y. He L. L. Sun X. Dresselhaus M. S. 1998Appl. Phys. Lett., 72, 3282
Cassell A. M. Raymakers J. A. Kong J. Dai H. J. 1999Phys. Chem. B., 103, 6484
J. Colomer F. Stephan C. Lefrant S. Van Tendeloo G. Willems I. Konya Z. Fonseca A. Laurent C. Nagy J. B. 2000Chem. Phys. Lett., 317, 83
Su M. Zheng B. Liu J. 2000Chem. Phys. Lett., 322, 321
Bronikowski M. J. Willis P. A. Colbert D. T. Smith K. A. Smalley R. E. 2001J. Vac. Sci. Technol. A, 19, 1800
Li Q. Hao Y. Yan C. Jin Z. Liu Z. 2002J. Mater. Chem., 12, 1179
Hornyak G. L. Grigorian L. Dillon A. C. Parilla P. A. Jones K. M. Heben M. J. 2002J. Phys. Chem. B., 106, 2821
Wagg L. M. Hornyak G. L. Grigorian L. Dillon A. C. Jones K. M. Blackburn J. Parilla P. A. Heben M. J. 2005J. Phys. Chem. B., 109, 10435
Hafner J. H. C. Cheung L. Oosterkamp T. H. Lieber C. M. 2001J. Phys. Chem. B., 105, 743
Mahan A. H. Alleman J. L. Heben M. J. Parilla P. A. Jones K. M. Dillon A. C. 2002Appl. Phys. Lett., 81, 4061
Chiang I. W. Brinson B. E. Huang A. Y. Willis P. A. Bronikowski M. J. Margrave J. L. Smalley R. E. Hauge R. H. 2001J. Phys. Chem. B., 105, 8297
Liu B. L. Ren W. C. Gao L. B. Li S. S. Pei S. F. Liu C. Jiang C. B. Cheng H. M. 2009J. Am. Chem. Soc., 131, 2082
Ebbesen T. W. Ajayan P. M. 1992Nature., 358, 220
Dillon A. C. Mahan A. H. Parilla P. A. Alleman J. L. Heben M. J. Jones K. M. Gilbert K. E. H. 2003Nano Lett., 3, 1425
Wang W. D. Serp P. Kalck P. Silva C. G. Faria J. L. 2008Mater. Res. Bull., 43, 958
Ribaya B. P. Leung J. Brown P. Rahman M. Nguyen C. V. 2008Nanotechnology. 2008, 19
Bokobza L. 2007Polymer, 48, 4907
Raffaelle R. P. Landi B. J. Harris J. D. Bailey S. G. Hepp A. F. 2005Materials Science and Engineering B-Solid State Materials for Advanced Technology., 233
Ngo Q. Petranovic D. Krishnan S. Cassell A. M. Ye Q. Li J. Meyyappan M. Yang C. Y. 2004IEEE Trans. Nanotechnol., 3, 311
Gong K. P. Zhang M. N. Yan Y. M. Su L. Mao L. Q. Xiong Z. X. Chen Y. 2004Anal. Chem., 76, 6500
Gomes H. T. Samant P. V. Serp P. Kalck P. Figueiredo J. L. Faria J. L. 2004Appl. Catal., B., 54, 175
Lueking A. Yang R. T. J. 2005Catal., 206, 165
Qin L. C. 1997J. Mater. Sci. Lett., 16, 457
Y.-Y. Fan, F. Li, H.-M. Cheng, G. Su, Y.-D. Yu, Z.-H. Shen. (1998.) J. Mater. Res., 13, 2342
Marangoni R. Serp P. Feurer R. Kihn Y. Kalck P. Vahlas C. 2001Carbon., 39, 443
Andrews R. Jacques D. Rao A. M. Derbyshire F. Qian D. Fan X. Dickey E. C. Chen J. 1999Chem. Phys. Lett., 303, 467
Endo M. Takeuchi K. Igarashi S. Kobori K. Shiraishi M. Kroto H. W. 1993J. Phys. Chem. Sol., 54, 1841
Jose-Yacaman M. Miki-Yoshida M. Rendon L. Santiesteban J. G. 1993Appl. Phys. Lett., 62, 202
Ivanov V. Nagy J. B. Lambin P. Lucas A. Zhang X. B. Zhang X. F. Bernaerts D. Van Tendeloo G. Amelinckx S. Van Landuyt J. 1994Chem. Phys. Lett., 223, 329
Thong J. T. L. Oon C. H. Eng W. K. Zhang W. D. Gan L. M. 2001Appl. Phys. Lett., 79, 2811
Tang D. S. Xie S. S. Pan Z. W. Sun L. F. Liu Z. Q. Zou X. P. Li Y. B. Ci L. J. Liu W. Zou B. S. Zhou W. Y. 2002Chem. Phys. Lett., 356, 563
Lee C. J. Kim D. W. Lee T. J. Choi Y. C. Park Y. S. Kim W. S. Lee Y. H. Choi W. B. Lee N. S. Kim J. M. Choi Y. G. Yu S. C. 1999Appl. Phys. Lett., 75, 1721
Xie S. Li W. Pan Z. Chang B. Sun L. 2000Mater. Sci. Eng. A., 286, 11
Li Y. J. Sun Z. Lau S. P. Chen G. Y. Tay B. K. 2001Appl. Phys. Lett., 79, 1670
Qin L. C. Zhou D. Krauss A. R. Gruen D. M. 1998Appl. Phys. Lett., 72, 3437
Chen M. C. Chen M. C. Chen F. 2002J. Mater. Sci., 37, 3561
Choi Y. C. Bae D. J. Lee Y. H. Lee B. S. G. Park S. Choi W. B. Lee N. S. Kim J. M. J. 2000Vac. Sci. Technol. A., 18, 1864
Chung S. J. Lim S. H. Lee C. H. Jang J. 2001Diamond Relat. Mater., 10, 248
Ho G. W. Wee A. T. S. Lin J. Tiju W. C. 2001Thin Solid Films., 388, 73
Wang H. Lin J. Huan C. H. A. Dong P. He J. Tang S. H. Eng W. K. Thong T. L. J. 2001Appl. Surf. Sci., 181, 248
Res., 15 Zhang Q. Yoon S. F. Ahn J. Gan B. Rusli M. Yu B. (1749 Mater J.
Yoon H. J. Kang H. S. Shin J. S. Son K. J. Lee C. H. Kim C. O. Hong J. P. Cha S. N. Song B. G. Kim J. M. Lee N. S. Physica B.
Woo Y. S. Jeon D. Y. Han I. T. Lee N. S. Jung J. E. Kim J. M. 2002Diamond Relat. Mater., 11, 59
Lee H. Y. Kang S. Lee P. S. J. Lee Y. 2002J. Alloys Compd., 330, 569
Bower C. Zhou O. Zhu W. Werder D. J. Jin S. 2000Appl. Phys. Lett., 77, 2767
Park K. H. Lee K. M. Choi S. Lee S. Koh K. H. 2001J. Vac. Sci. Technol. B., 19, 946
Ono T. Miyashita H. Esashi M. 2002Nanotechnology., 13, 62
J.-h Han. B. Moon S. Yang W. S. J. Yoo B. Park C. Y. 2000Surf. Coat. Technol., 131, 93
Ren Z. F. Huang Z. P. Xu J. W. Wang J. H. Bush P. Siegal M. P. Provincio P. N. 1998Science., 282, 1105
C. Chen F. C. Lin L. C. Wang M. J. 2002Appl. Phys., 41, L67
Du G. X. Zhu Z. P. Zhang L. D. Song J. L. 2010Mater. Lett., 64, 1179
The Chemistry of Nanomaterials: Synthesis, Properties and Applications, JohnWiley, Rao C. N. R. Müller C. A. K. Achim 2004
Wildgoose G. G. Banks C. E. Compton R. G. 2006Small., 2, 182
Georgakilas V. Gournis D. Tzitzios V. Pasquato L. Guldi D. M. Prato M. 2001J. Mater. Chem., 17, 2679
Hu X. G. Dong S. J. 2008J. Mater. Chem., 18, 1279
Vairavapandian D. Vichchulada P. M. D. 2008Lay. Anal. Chim. Acta., 626, 119
Peng X. Chen J. Misewich J. A. Wong S. S. 2009Chem. Soc. Rev., 38, 1076
Chiang I. W. Smalley R. E. Margrave J. L. Hauge R. H. 2001J. Phys. Chem. B., 106, 1157
Tohji T. Takahashi H. Shinoda Y. Shimizu N. Jeyadevan B. Matsuoka I. Saito Y. Kasuya A. Ohsuna T. Hiraga K. Nishina Y. 1996Nature., 383, 679
Dujardin E. E. Krishnan A. Treacy M. M. J. 1998Adv. Mater., 10, 611
Xu H. Y. Hauge R. H. Smalley R. E. 2005Nano Lett., 5, 163
Fang H. T. Liu C. G. Liu C. Li F. Liu M. Cheng H. M. 2004Chem. Mater., 16, 5744
Murphy C. J. R. Cadek M. Mc Carthy B. Bent M. Drury A. 2002J. Phys. Chem. B., 106, 3087
Shen K. Curran S. Xu H. F. Rogelj S. Jiang Y. B. Dewald J. Pietrass T. 2005J. Phys. Chem. B., 109, 4455
Liu A. G. Dai H. Hafner J. H. Bradley R. K. Boul P. J. Lu A. Iverson T. She-limov K. Huffman C. B. Rodriguez-Macias F. Y. Shon S. Lee T. R. Colbert D. T. Smalley R. E. 1998Science., 280, 1253
Chen M. A. Hu H. Chen Y. Rao A. M. Eklund P. C. Haddon R. C. 1998Science., 282, 95
Fu W. Lin Y. Riddle L. A. Carroll D. L. Y. Sun P. 2001Nano Lett., 1, 439
Kamaras M. E. Hu H. Zhao B. Haddon R. C. 2003Science., 301, 1501
Strano C. A. Usrey M. L. Barone P. W. Allen M. J. Shan H. Kittrell C. Hauge R. H. Tour J. M. Smalley R. E. Dujardin T. W. Ebbesen A. Krishnan M. Treacy M. J. 2003Science., 301, 1519
Zheng A. Semke E. D. Diner B. A. Mc Lean R. S. Lustig S. R. Richardson R. E. Tassi N. G. 2003Nat. Mater., 2, 338
Chen Y. Wang D. Dai H. 2001J. Am. Chem. Soc., 123, 3838
J. Besteman O. Wiertz F. G. M. Heering H. A. Dekker C. 2003Nano Lett., 3, 727
Moore M. S. Haroz E. H. Hauge R. H. Smalley R. E. Schmidt J. Talmon Y. Nano Lett.
Fukushima A. Ishimura Y. Yamamoto T. Takigawa T. Ishii N. Aida T. 2003Science., 300, 2072
Wang H. C. J. Li Y. 2008ACS Nano., 2, 2540
Wang J. Y. Li Y. 2009J. Am. Chem. Soc., 131, 5364
Ajayan P. M. Lijima S. 1993Nature., 361, 333
Ajayan P. M. Ebbesen T. W. Ichihashi T. Iijima S. Tanigaki K. Hiura H. 1993Nature., 362, 522
Sloan J. Hammer J. Zwiefka-Sibley M. Green M. L. H. 1998Chem. Commun., 3, 347
Loebick C. Z. Majewska M. Ren F. Haller G. L. Pfefferle L. D. 2010J. Phys. Chem. C., 114, 11092
Jain D. Wilhelm R. 2007Carbon., 45, 602
Schnitzler M. C. Oliveira M. M. Ugarte D. Zarbin A. J. G. Chem 2003Phys. Lett., 381, 541
Monthioux M. Flahaut E. Cleuziou J. P. 2006J. Mater. Res., 21, 2774
Chen J. Hamon M. A. Hu H. Chen Y. S. Rao A. M. Ecklund P. C. Haddon R. C. 1998Science., 282, 95
Haremza J. M. Hahn M. A. Krauss T. D. Chen S. Calcines J. 2002Nano Lett., 2, 1253
G. Wang X. B. Zhang L. Z. Yu L. M. Qu Z. 2005Solid State Ionics., 176, 1169
Liu B. Chen J. H. Xiao C. H. Cui K. Z. Yang L. Pang H. L. Kuang Y. F. 2007Energy Fuels., 21, 1365
Kongkanand A. Dominguez R. M. Kamat P. V. 2007Nano Lett., 7, 676
Sainsbury T. Fitzmaurice D. 2004Chem. Mater., 16, 3780
Yang D. Q. Hennequin B. Sacher E. 2006Chem. Mater., 18, 5033
Guldi D. M. Rahman G. M. A. Jux N. Tagmatarchis N. Prato M. 2004Angew. Chem. Int. Ed., 43, 5526
Chen R. J. Zhang Y. Wang D. Dai H. 2001J. Am. Chem. Soc., 123, 3838
Murakami H. Nomura T. Nakashima N. 2003Chem. Phys. Lett., 378, 481
Satake A. Miyajima Y. Kobuke Y. 2005Chem. Mater., 17, 716
Rahman G. M. A. Guldi D. M. Campidelli S. Prato M. 2006J. Mater. Chem., 16, 62
Wang X. Liu Y. Qiu W. Zhu D. 2002J. Mater. Chem., 12, 1636
D’Souza F. Chitta R. Sandanayaka A. S. D. Subbaiyan N. K. D’Souza L. Araki Y. Ito O. 2007Chem.sEur. J., 13, 8277
Mu Y. Liang H. Hu J. Jiang L. Wan L. 2005J. Phys. Chem. B., 109, 22212
Georgakilas V. Tzitzios V. Gournis D. Petridis D. 2005Chem. Mater., 17, 1613
Zhou J. Zhou X. Sun X. Lib R. Murphy M. Ding Z. Sun X. T. Sham K. 2007Chem. Phys. Lett., 437, 229
Guldi D. M. Taieb H. Rahman G. M. A. Tagmatarchis N. Prato M. 2005Adv. Mater., 17, 871
Correa-Duarte M. A. Liz-Marza´n L. M. 2006J. Mater. Chem. 2006, 16, 22
Chen H. Donga S. 2006Talanta., 71, 1752
Ostranger J. W. Mamedov A. A. Kotov N. A. 2001J. Am. Chem. Soc., 123, 1101
Jiang K. Eitan A. Schadler L. S. Ajayan P. M. Siegel R. W. Grobert N. Mayne M. Reyes-Reyes M. Terrones H. Terrones M. 2003Nano Lett., 3, 275
Correa-Duarte M. A. Perez-Juste J. Sanchez-Iglesias A. Giersig M. 2005Angew. Chem. Int. Ed., 44, 4375
Hu X. Wang T. Qu X. Dong S. 2006J. Phys. Chem. B., 110, 853
Sun J. Gao L. 2006J. Electroceram., 17, 91
Sun J. Iwasa M. Gao L. Zhang Q. 2004Carbon., 42, 895
Stoffelbach F. Aqil A. Jerome C. Jerome R. Detrembleur C. 2005Chem. Commun., 4532
Guo D. J. Li H. L. 2004Electrochem. Commun. 2004, 6, 999
Day T. M. Unwin P. R. Wilson N. R. Macpherson J. V. 2005J. Am. Chem. Soc., 127, 10639
Guo D. J. Li H. L. 2004J. Electroanal. Chem., 573, 197
Y. 2004J. Phys. Chem. B., 108, 19255
Lin Y. Cui X. Yen C. Wai C. M. 2005J. Phys. Chem. B., 109, 14410
Sivakkumar S. R. Ko J. M. Kim D. Y. Kim B. C. Wallace G. G. 2007Electrochim. Acta., 52, 7377
Xie X. Gao L. 2007Carbon., 45, 2365
Huang X. P. Pan C. X. Huang X. T. 2007Mater. Lett., 61, 934
Huang B. Huang R. Jin D. Ye D. 2007Catal. Today., 126, 279
Moriguchi I. Hidaka R. Yamada H. Kudo T. Murakami H. Nakashima N. 2006Adv. Mater., 18, 69
Sun J. Gao L. Iwasa M. 2004Chem. Commun., 832
Frank O. Kalbac M. Kavan L. Zukalova M. Prochazka J. Klementova M. Dunsch L. 2007Phys. Status Solidi., 244, 4040
K. He X. Q. Wu F. X. Zhang G. X. Wang L. 2006J. Electrochem. Soc., 153, A1568
I. Kim H. J. Kim H. Y. Lee H. K. Kim B. 2005J. Electrochem. Soc., 152, A2170
Kim J. D. Kang B. S. Noh T. W. J. Yoon G. Baik S. I. Y. Kim W. 2005J. Electrochem. Soc., 152, D23
Wang C. Waje M. Wang X. Tang J. M. Haddon R. C. Yan Y. 2004Nano Lett., 4, 345
Sol Gel Sciences The Physics and Chemistry of Sol Gel Processing; Academic Press: New York, Brinker C. J. Scherer G. W. 1990
Vincent P. Brioude A. Journet C. Rabaste S. Purcell S. T. Brusq J. L. Plenet J. C. 2002J. Non-Cryst. Solids., 311, 130
Jitianu A. Cacciaguerra T. Benoit R. Delpeux S. Beguin F. Bonnamy S. 2004Carbon., 42, 1147
Jitianu A. Cacciaguerra T. Berger M. H. Benoit R. Beguin F. Bonnamy S. 2004J. Non-Cryst. Solids., 34546, 596
Zhao L. P. Gao L. 2004Carbon., 42, 1858
Eder D. Windle A. H. 2008J. Mater. Chem., 18, 2036
Yu Y. Yu J. C. J. Yu G. Y. Kwok C. Y. Che K. J. Zhao C. Ding L. W. Ge K. P. Wong K. 2005Appl. Catal., A., 289, 186
Song H. Qiu X. Li F. Zhu W. Chen L. 2007Electrochem. Commun. 2007, 9, 1416
W. Han Q. Zettl A. 2003Nano Lett., 3, 681
Bai J. Y. Xu Z. D. Zheng Y. F. 2006Chem. Lett., 35, 96
Li Y. Ding J. Chen J. Xu C. Wei B. Liang J. Wu D. 2002Mater. Res. Bull., 37, 313
Liang Y. X. Chen Y. J. Wanga T. H. 2004Appl. Phys. Lett., 85, 666
Chen M. H. Huang Z. C. Wu G. T. Zhu G. M. You J. K. Lin Z. G. 2003Mater. Res. Bull., 38, 831
B. Wei Y. M. Hsu C. P. Su G. H. Lin M. R. Wu J. H. Lai J. 2004Sens. Actuators, B., 101, 81
Wang W. D. Serp P. Kalck P. Silva C. G. Faria J. L. 2008Mater. Res. Bull., 43, 958
Wang W. D. Serp P. Kalck P. Faria J. L. Mol J. 2005Catal. A: Chem., 235, 194
Wang W. D. Serp P. Kalck P. Faria J. L. Appl Catal. B.
Arabale G. Wagh D. Kulkarni M. Mulla I. S. Vernekar S. P. Vijayamohanan K. Rao A. M. 2003Chem. Phys. Lett., 376, 207
Park J. H. Ko J. M. Parka O. O. 2003J. Electrochem. Soc., 150, A864
Lee J. Y. Liang K. Ana K. H. Lee Y. H. 2005Synth. Met., 150, 153
R. Wu J. J. Wu G. M. Yu R. T. K. T. C. Yeh T. 2008Sens. Actuators, B., 131, 306
Cao L. Scheiba F. Roth C. Schweiger F. Cremers C. Stimming U. Fuess H. Chen L. Zhu W. Qiu X. 2006Angew. Chem. Int. Ed., 45, 5315
Eder D. Windle A. H. 2008Adv. Mater., 20, 1787
Hernadi K. Ljubovic E. Seo J. W. Forro L. 2003Acta Mater., 51, 1447
Vietmeyer F. Seger B. Kamat P. V. 2007Adv. Mater., 19, 2935
Jiang L. Gao L. 2005Mater. Chem. Phys., 91, 313
Yoshimura M. Byrappa K. J. 2008Mater. Sci., 43, 2085
Menzel R. Peiro´ A. M. Durrant J. R. Shaffer M. S. P. 2006Chem. Mater., 18, 6059
Byrappa K. Dayananda A. S. Sajan C. P. Basavalingu B. Shayan M. B. Soga K. Yoshimura M. 2008J. Mater. Sci., 43, 2348
Lee Y. Song H. J. Shin H. S. Shin H. J. Choi H. C. 2005Small., 1, 975
Huang Y. Lin J. Ding X. X. Tang C. Gu C. Z. Qi S. R. 2007Mater. Lett., 61, 697
Zhang W. D. 2006Nanotechnology., 17, 1036
Yu Y. Ma Huang L. L. W. Y. Li J. L. Wong P. K. Yu J. C. 2005J. Solid State Chem., 178, 1488
Yu Y. Ma Huang L. L. W. Y. Du F. P. Yu J. C. Yu J. G. Wang J. B. Wong P. K. 2005Carbon., 43, 670
Jia B. P. Gao L. 2007J. Sun. Carbon., 45, 1476
Fu L. Liu Z. M. Liu Y. Q. Han B. X. Wang J. Q. Hu P. A. Cao L. C. Zhu D. B. 2004Adv. Mater., 16, 350
Sun Z. Y. Zhang X. R. Han B. X. Wu Y. Y. An G. M. Liu Z. M. Miao S. D. Miao Z. J. 2007Carbon., 45, 2589
Sun X. Chu Y. Wang D. W. Du J. H. Zhang B. Y. Wang F. P. 2007Rare Metals., 26, 191
Sun Z. Liu Z. Han B. G. 2007An. Mater. Lett., 61, 4565
Sun Z. Yuan H. Liu Z. Han B. Zhang X. 2005Adv. Mater., 17, 2993
Sun Z. Liu Z. Han B. Miao S. Du J. Miao Z. 2006Carbon., 44, 888
Kim H. Sigmund W. 2002Appl. Phys. Lett., 81, 2085
Ye J. S. Cui H. F. Liu X. Lim T. M. Zhang W. D. Sheu F. S. 2005Small., 1, 560
Zhu Y. W. Elim H. I. Foo Y. L. Yu T. Liu Y. J. Ji W. Lee J. Y. Shen Z. X. Wee A. T. S. Thong J. T. L. Sow C. H. 2006Adv. Mater., 18, 587
Jin F. Liu Y. Day C. M. 2007Appl. Phys. Lett., 90, 143114
W. Fang C. Chyan O. C. Sun L. C. Wu T. C. Chen P. K. Chen H. L. Chen C. J. Huang H. 2007Electrochem. Commun., 9, 239
Ikuno T. Yasuda T. Honda S. I. Oura K. Katayama M. Lee J. G. Mori H. J. 2005Appl. Phys., 98, 114305
Ikuno T. Katayama M. Kamada K. Honda S. Lee J. G. Mori H. Oura K. 2003J. Appl. Phys. Lett., 42, L1356
Kuang Q. Li S. F. Xie Z. X. Lin S. C. Zhang X. H. Xie S. Y. Huang R. B. Zheng L. S. 2006Carbon., 44, 1166
Deng G. H. Xiao X. Chen J. H. Zeng X. B. He D. L. Kuang Y. F. 2005Carbon., 43, 1557
Acta., 2959 Fan Z. Chen J. Cui K. Sun F. Xu Y. Kuang Y. (200 Electrochim
Chrissanthopoulos A. Baskoutas S. Bouropoulos N. Dracopoulos V. Tasis D. Yannopoulos S. N. 2007Thin Solid Films., 515, 8524
Lazareck A. D. T. Kuo F. Xu J. M. Taft B. J. Kelley S. O. Cloutier S. G. 2006Appl. Phys. Lett., 89, 103109
Lazareck A. D. Cloutier S. G. T. Kuo F. Taft B. J. Kelley S. O. Xu J. M. 2006Nanotechnology., 17, 2661
Liu J. Li X. Dai L. 2006Adv. Mater., 18, 1740
Ho Y. M. Liu J. W. Qi J. L. Zheng W. T. 2008J. Phys. D: Appl. Phys., 41, 665308
Gomathi A. Vivekchand S. R. C. Govindaraj A. Rao C. N. R. 2005Adv. Mater., 17, 2757
Javey A. Kim H. Brink M. Wang Q. Ural A. Guo J. Mcintyre P. Mc Euen P. Lundstrom M. Dai H. 2002Nat. Mater., 1, 241
Ren N. Dong A. G. Cai W. B. Zhang Y. H. Yang W. L. Huo S. J. Chen Y. Xie S. H. Gao Z. Tang Y. 2004J. Mater. Chem., 14, 3548
Qiao J. Tang S. N. Tiana Y. N. Shuang S. M. Dong C. Choi M. M. F. 2009Sens. Actuators B., 138, 402
Mo G. Q. Ye J. S. Zhang W. D. 2009Electrochimica Acta., 55, 511
Ma Tian W. D. B. 2010Bioelectrochemistry., 78, 106
Zhu K. N. Qin H. Y. Liu B. H. Li Z. P. 2011J. Power Sources., 196, 182
Hirayama T. Manako T. Imai H. 2008e-J. Surf. Sci. Nanotech., 6, 237
Jimenez I. Centeno M. A. Scotti R. Morazzoni F. Cornet A. Morante J. R. 2003J. Electrochem. Soc., 150, H72
Fru B. °hberger M. Grunze D. J. Dwyer 1996Sens. Actuators, B., 31, 167
Wu N. L. Wang S. Y. Rusakova I. A. 1999Science., 285, 1375
Collins P. G. Bradley K. Ishigami M. Zettl A. 2000Science., 287, 1801
Sinha N. Ma Yeow J. Z. J. T. W. Nanosci J. 2006Nanotechnol., 6, 573
Kong J. Franklin N. R. Zhou C. Chapline M. G. Peng S. Cho K. Dai H. 2000Science., 287, 622
Sun Z. Zhang X. Na N. Liu Z. Han B. An G. 2006J. Phys. Chem. B., 110, 13410
Van Hieu N. Thuy L. T. B. Chien N. D. 2008Sens. Actuators, B., 129, 888
Liu J. Guo Z. Meng F. Jia Y. Liu J. 2008J. Phys. Chem. C., 112, 6119
Chen Y. Zhu C. Wang T. 2006Nanotechnology., 17, 3012
Jiang L. C. Zhang W. D. 2010Biosens. Bioelectron., 25, 1402
Liu Z. Wang J. Xie D. Chen G. 2008Small., 4, 462
Fang B. Zhang C. H. Zhang W. Wang G. F. 2009Electrochim. Acta., 55, 178
Conway B. E. 1991J. Electrochem. Soc., 138, 1539
Niu C. Sichel E. K. Hoch R. Moy D. Tennet H. 1997Appl. Phys. Lett., 70, 1480
Lota G. Lota K. Frackowiak E. 2007Electrochem. Commun., 9, 1828
Yi W. Yu S. G. Lee W. T. Han I. T. Jeong J. T. Woo Y. S. Lee J. H. Jin S. W. Choi W. B. Heo J. N. Jeon D. Kim J. M. 2001J. Appl. Phys., 89, 4091
Nam K. W. Kim K. H. Lee E. S. Yoon W. S. Yang X. Q. Kim K. B. 2008J. Power Sources., 182, 642
Subramanian V. Zhu H. W. Wei B. Q. 2006Electrochem. Commun., 8, 827
Deng M. G. Yang B. C. Zhang Z. A. Hu Y. D. 2005J. Mater. Sci., 40, 1017
Zhang H. Cao G. Wang Z. Yang Y. Shi Z. 2008Nano Lett., 8, 2664
Reddy A. L. M. Shaijumon M. M. Gowda S. R. Ajayan P. M. 2009Nano Lett., 9, 1002
G. Wu M. A. Wang R. M. Zhang X. H. Yang Y. Zhou B. Shen J. J. 2008Sol Gel Sci. Technol., 46, 79
W. Fang C. 2008J. Phys. Chem. C., 112, 11552
W. Fang C. K. Chen H. L. Chen C. 2007Nanotechnology., 18, 485716